Vibration analysis of a singlelayered graphene sheet embedded in viscoPasternak’s medium using nonlocal elasticity theory
Ashraf M. Zenkour^{1}
^{1}Department of Mathematics, Faculty of Science, King Abdulaziz University, Jeddah 21589, Saudi Arabia
^{1}Department of Mathematics, Faculty of Science, Kafrelsheikh University, Kafrelsheikh 33516, Egypt
Journal of Vibroengineering, Vol. 18, Issue 4, 2016, p. 23192330.
https://doi.org/10.21595/jve.2016.16585
Received 28 October 2015; received in revised form 14 January 2016; accepted 18 January 2016; published 30 June 2016
The vibration analysis of a singlelayered graphene sheet (SLGS) embedded in viscoelastic medium is presented by using the nonlocal elasticity theory. The medium is considered by adding the damping to the usual foundation model which characterized by the linear Winkler’s modulus and Pasternak’s (shear) foundation modulus. The governing dynamical equation is obtained and solved for simplysupported SLGSs. The effects of many parameters like nonlocal parameter, aspect ratio, WinklerPasternak’s foundation, damping coefficient, and mode numbers on the vibration frequencies of the SLGSs are investigated in detail. The present results are compared with the corresponding available in the literature. Additional results are tabulated and plotted for sensing the effect of all used parameters and to investigate the viscoPasternak’s parameters for future comparisons.
Keywords: nonlocal elasticity theory, graphene sheet, vibration frequencies, viscoPasternak’s medium.
1. Introduction
In recent years, the elements of nanostructures such as nanobeams, nanotubes and nanoplates are commonly used as components in nanoelectromechanical devices and other applications. Some of these nanostructured materials such as singlelayered graphene sheets (SLGSs), multilayered graphene sheets (MLGSs), fullerenes and different types of carbon nanotubes (CNTs) are fundamental building blocks of nanotechnology. Hence, accurate prediction of their thermomechanical behaviors becomes essential for engineering design and manufacture. But, controlled experiments on nanoscale are difficult to perform. The unique properties of the SLGSs or MLGSs make them very attractive in many scientific research aspects. Some remarkable mechanical properties of the GSs reveal that they have potential for creating novel ultrastrength composite materials [1, 2]. The GSs are mostly used in polymer composites as embedded structures to fortify them. Furthermore, the potential applications of the SLGSs as mass sensors and atomistic dust detectors have been investigated [3].
The notions of continuum mechanics have attracted a great deal of attention of many researchers to treat structures at the scale of nanometer. The classical continuum mechanics approaches are widely used but theory cannot predict the size effect. Successful applications of the classical continuum modeling to the vibration frequencies of CNTs and GSs have been reported by a number of research workers [412]. However, the classical continuum mechanics is scale independent which makes its applicability to the smallscale nanomaterials somewhat questionable. The size effects are recognized to become more pronounced as the dimensions of nanostructures become very small. It has been suggested that the nonlocal continuum theory presented by Eringen [1316] should be integrated in the continuum models for accurate prediction of nanostructures mechanical behaviors [17]. The nonlocal Eringen’s theory is based on this assumption that the stress at a material point is considered as a function of the strain field at all material points in the continuum body. The interatomic forces and atomic length scales directly come to the constitutive relations as material parameters.
The extension of continuum mechanics to accommodate the size dependence of nanomaterials becomes another topic of major concern. Application of nonlocal continuum mechanics allowing for the small scale effects to vibration frequency analysis of nanomaterials has been also suggested by some other research workers in the study of nanostructures [1843]. However, the inclusion of the damping effect as a third foundation parameter is rare in the literature. Arani et al. [44] have used the nonlocal elasticity theory to study the vibration analysis of the coupled system of DLGSs embedded in a viscoPasternak foundation. Pouresmaeeli et al. [45] have studied the vibration characteristics of a simplysupported viscoelastic nanoplate using the nonlocal plate theory by including the effect of viscoelastic foundation. Mohammadi et al. [46] have studied the vibration behavior of circular and annular GSs embedded in a viscoPasternak foundation and coupled with temperature change and under inplane preload. Karličić et al. [47] have analyzed the free transverse vibration of a viscoelastic multinanoplate system embedded in a viscoelastic medium taking into account smallscale effects by using the nonlocal theory. Goodarzi et al. [48] have studied the free vibration behavior of rectangular graphene sheet under shear inplane load. Hashemi et al. [49] have used the nonlocal theory to study the free transverse vibration of a nonlocal viscoelastic double graphene sheets coupled with viscoPasternak layer. Zenkour [50] has presented the nonlocal transient thermal analysis of a SLGS embedded in viscoelastic medium.
The vibration frequency analysis of a SLGS embedded in a viscoPasternak’s medium is presented to display various characters. The governing equation is obtained and solved analytically for a simplysupported SLGS. The effects of different parameters on the natural vibration frequencies are investigated. Sample results are tabulated and plotted for sensing the effect of all used parameters and to investigate the viscoPasternak’s parameters for future comparisons.
2. Basic equation of singlelayered graphene sheet (SLGS)
Let us consider a singlelayered graphene sheet (SLGS) of length $a$, width $b$ and uniform thickness $h$ as shown in Fig. 1. The SLGS is made of a homogeneous isotropic and linearly elastic material with Young’s modulus $E$, Poisson’s ratio $\nu $, shear modulus $G$ and material density $\rho $.
Fig. 1. A continuum plate model of a singlelayered graphene sheet embedded in a viscoelastic medium
2.1. The viscoWinklerPasternak foundations
The twoparameter Pasternak’s model is the most natural extension to the oneparameter Winkler’s model. It considers a shear interaction between the spring elements by connecting the ends of the springs to a plate of an incompressible shear layer. The present SLGS is embedded in a homogeneous threeparameter viscoelastic medium. The foundation model is characterized by the linear Winkler’s modulus ${K}_{1}$, the Pasternak’s (shear) foundation modulus ${K}_{2}$, and the damping coefficient ${c}_{t}$ of the viscoelastic medium. Taking into account the unbonded contact between the SLGS and medium, the interaction follows the threeparameter viscoPasternaktype foundation model as:
where $w$ is the transverse displacement and ${\nabla}^{2}$ is the Laplacian (secondorder spatial gradient). Here, we have introduced the SLGS length $a$ in Eq. (1) for maintaining the dimension of ${K}_{1}$ and ${K}_{2}$ to be the same. If the foundation is modelled as the viscoWinkler foundation, the coefficient ${K}_{2}$ in Eq. (1) is zero. The viscosity term may be omitted by setting ${c}_{t}=\text{0}$ to get the analysis of the SLGS embedded in pure elastic medium.
2.2. Nonlocal classical plate theory
The most general form of the constitutive relation in nonlocal elasticity theory involves an integral over the entire region of interest. The integral contains a nonlocal kernel function, which describes the relative influence of the strains at the various locations of the body on the stress at the material point under consideration. Specifically, the constitutive equation of nonlocal elasticity for homogenous and isotropic elastic solids read:
where ${\sigma}_{ij}$ is the nonlocal stress tensor, $V$ is the volume occupied by the elastic body, $\leftx{x}^{\text{'}}\right$ denotes distance in Euclidean space, and the nonlocal kernel $\alpha \left(\leftx{x}^{\text{'}}\right\right)$ accounts for the effect of the strain at the point ${x}^{\text{'}}$ on the stress at the point $x$ in the elastic body.
The quantity ${\tau}_{kl}\left({x}^{\text{'}}\right)$ denotes the local stress tensor for which the standard local constitutive equation is adopted, i.e.:
where ${\epsilon}_{kl}\left({x}^{\text{'}}\right)$ is the classical local strain tensor at ${x}^{\text{'}}$, and $\lambda $ and $\mu $ being Lamé’s constants.
The small straindisplacement relations are given by the usual relations:
where ${u}_{l}\left({x}^{\text{'}}\right)$ is the displacement vector at a reference point ${x}^{\text{'}}$ in the body. For an appropriate form of the nonlocal kernel [1316], it turns out that the nonlocal internal constitutive relation given by Eq. (2) can be inverted to yield the following pseudolocal constitutive equation of gradient type:
The parameter $l$ is an internal characteristic length (e.g., lattice parameter, granular distance), and ${e}_{0}$ is a material constant determined by experiment or by matching dispersion curves of plane waves with those of atomic lattice dynamics. One may see that when the internal characteristic length $l$ is neglected, i.e. the particles of the medium are considered to be continuously distributed and interacting without longrange forces, $l{e}_{0}$ is zero, and Eq. (5) reduces to the constitutive equation of classical local elasticity theory.
The displacement field models are chosen such that to ensure zero transverse shear stresses on top and bottom surfaces of the thicker plate. For the present very thin SLGS, it is sufficient and efficient to use the classical thin plate theory. The displacement field can be written as:
where ${u}_{1}$, ${u}_{2}$, and ${u}_{3}$ are the displacements in the $x$, $y$, and $z$ directions, $u$, $v$, and $w$ are the midplane displacements. Here $u$ and $v$ are the inplane displacements while $w$ is the transverse displacement (deflection).
By substituting the displacement relations given in Eq. (6) into the straindisplacement equations of elasticity, the normal and shear strain components are obtained as:
The corresponding stressstrain relationships in the isotropic SLGS coordinates can be expressed as:
where $\xi ={\left(l{e}_{0}\right)}^{2}$ represents the nonlocal parameter.
2.3. Equation of motion
The governing equation of motion in the transverse deflection $w$ only can be obtained by using the dynamic version of the principle of virtual displacements in the form:
where ${M}_{xx}$, ${M}_{xy}$, and ${M}_{yy}$ are the basic components of stress couples. They can be obtained by integrating Eq. (8) over the thickness of the plate as:
In addition, ${I}_{0}$ and ${I}_{2}$ represent the mass moments of inertia and are defined as:
Using the stressstrain relationship, Eq. (8), and the stress resultants definition, Eq. (10), with the aid of Cauchy’s relations, Eq. (7), we can express stress resultants in terms of transverse displacement as follows:
The substitution of Eq. (12) into Eq. (9) gives the following nonlocal governing partial differential equation in terms of transverse flexural displacement without the effect of the external load ($q=0$):
where $D=E{h}^{3}/12\left(1{\nu}^{2}\right)$ is the flexural rigidity of the SLGS.
3. Solution of nonlocal vibration
The determination of natural frequencies is of fundamental importance in the design of many nanostructuers. The vibration formulation begins by assuming a solution of the displacement field. In particular, time harmonic waves are sought and it is assumed that the model is unbounded in $x$ and $y$ directions. Thus, the assumed form of the displacement is combinations of Fourier transform in $x$ and $y$ directions and Fourier transform in time $t$:
where ${\omega}_{mn}$ is the circular frequency and $m$, $n$ are the wavenumbers along $x$ and $y$ directions, respectively, ${\lambda}_{m}=m\pi /a$, ${\mu}_{n}=n\pi /b$, and $\mathrm{i}=\sqrt{1}$.
To illustrate the preceding structural analysis, a variety of sample problems is considered. Whenever possible, comparisons are made with available solutions in the literature.
Substituting Eq. (14) into Eq. (13) we get:
where:
$C=D{\left({\lambda}_{m}^{2}+{\mu}_{n}^{2}\right)}^{2}\left[1+\xi \left({\lambda}_{m}^{2}+{\mu}_{n}^{2}\right)\right]\left[{K}_{1}+{K}_{2}{a}^{2}\left({\lambda}_{m}^{2}+{\mu}_{n}^{2}\right)\right].$
Eq. (15) represents the frequency equation for the SLGS and its solution for ${\omega}_{mn}$ is given by:
4. Numerical results and discussions
It is to be noted that, we get the equation of vibrations of the SLGSs using local theory sheets by setting the value of $\xi =\text{0}$ in Eq. (13). Correspondingly, the vibration frequencies of the local graphene are obtained. The fundamental frequencies for the present SLGSs are obtained with and without the inclusion of nonlocal parameter $\xi $. In what follows we will use the following dimensionless variables:
where ${k}_{1}$ and ${k}_{2}$ are the foundation parameters.
For the sake of comparison, we will study the effect of nonlocal parameter. For this purpose, the frequency ratio (FR) is defined as:
Properties of the graphene sheet in the validation analysis are considered in Table 1 [23]. The comparison of the results for vibration of nonlocal square SLGS between the present work and Refs. [23, 28, 29, 32] is presented in Table 2 with $a=b=\mathrm{}$10 nm and $h=\mathrm{}$0.34 nm and without the inclusion of viscoPasternake medium. The present frequency ratio is the same as those presented in the literature. Now, let us consider some numerical examples to put into evidence the effect of the aspect ratio $a/b$, the mode numbers $m$ and $n$, the foundation parameters ${k}_{1}$ and ${k}_{2}$, and the viscous damping coefficient ${c}_{t}$ on the vibration frequency of the present SLGS.
Table 1. Properties of the graphene sheet
$E$ (TPa)

$\nu $

$\rho $ (kg/m^{3})

$\alpha $ 10^{6}K^{1}

1.06

0.25

2250

1.1

Table 2. Comparison of the results for vibration of nonlocal square SLGS between the present work and Refs. [23, 28, 29, 32] ($a=b=\mathrm{}$10 nm and $h=$0.34 nm)
$\xi $ (nm^{2})

$\omega $ (GHz)

${\omega}_{NL}/{\omega}_{L}$


Present

[23]

[28]

[29]

[32]


0

0.19990

1

1

1

1

1

1

0.18268

0.91386

0.9139

0.9139

0.9139

0.9139

2

0.16926

0.84673

0.8467

0.8468

0.8466

0.8467

3

0.15843

0.79251

0.7925

0.7926

0.7926

0.7925

Benchmark results are presented in Table 3 for future comparison with other investigators. The effects of the nonlocal parameter $\xi $, viscous damping coefficient ${c}_{t}$, Winkler’s parameter ${k}_{1}$, Pasternak’s parameter ${k}_{2}$, and the mode number $n$ on the frequency $\omega $ of SLGSs are discussed. Table 3 shows that the SLGS not embedded in viscoPasternak’s medium gives the smallest frequencies $\omega $. The frequencies increase as the mode number $n$ increases and as the nonlocal parameter $\xi $ decreases. The SLGSs embedded in threeparameter (viscoPasternak’s) medium give frequencies smaller than those of SLGSs embedded in twoparameter (WinklerPasternak’s) medium. For SLGSs embedded in threeparameter medium, the frequencies increase with the increase of the foundation parameters ${k}_{1}$ and ${k}_{2}$ and with the decrease of the viscous damping coefficient ${c}_{t}$.
Additional plots are prepared in Figs. 26 by using the real value of the dimensionless frequency parameter $\omega $. The computations are carried out (except otherwise stated) for $m=1$, $a=2b$, $b=$10 nm, $h=\mathrm{}$0.34 nm, ${k}_{1}=$50 nN, ${k}_{2}=$10 nN, $\xi =$1 nm^{2}, and ${c}_{t}=$0.1 nN. Different values are given to the viscoPasternak’s parameters ${c}_{t}$, ${k}_{1}$, and ${k}_{2}$, and the aspect ratio $a/b$ of the SLGS. Here, we will discuss also the effect of the nonlocal parameter $\xi $ and the mode numbers $m$ and $n$.
Fig. 2 plots the natural frequencies $\omega $ vs the nonlocal parameter $\xi $ for different viscous damping coefficients ${c}_{t}$, foundation parameters ${k}_{1}$ and ${k}_{2}$, aspect ratios $a/b$, and mode numbers $m$ and $n$. The frequency increases with the increase of the foundation parameters ${k}_{1}$ and ${k}_{2}$, aspect ratios $a/b$ and mode numbers $m$ and $n$. However, the frequency decreases with the increase of the viscous damping coefficients ${c}_{t}$. The variation of $\omega $ is highly sensitive to the variation of all parameters.
Fig. 3 shows the variation of natural frequencies $\omega $ vs the viscous damping coefficient ${c}_{t}$ for different nonlocal parameters $\xi $, foundation parameters ${k}_{1}$ and ${k}_{2}$, aspect ratios $a/b$, and mode numbers $m$ and $n$. Once again, the frequency increases with the increase of the foundation parameters ${k}_{1}$ and ${k}_{2}$ and mode numbers $m$ and $n$. However, the frequency decreases as the nonlocal parameter $\xi $ increases. For lower values of ${c}_{t}$, the frequency increases as $a/b$ increases while $\omega $ decreases as $a/b$ increases for higher values of ${c}_{t}$. In fact, the frequencies may be vanished for higher values of the viscous damping coefficient ${c}_{t}$.
Table 3. Natural frequencies $\omega $ (GHz) of nonlocal square SLGS ($m=$ 1, $a=b=$ 10 nm and $h=$ 0.34 nm)
$\xi $

${c}_{t}$

${k}_{1}$

${k}_{2}$

$n$


1

2

3

4

5


0

0

0

0

0.19990

0.49905

0.99574

1.68721

2.56964

0

0

50
100
200

10
20
30

0.54193
0.73987
0.92327

0.89714
1.16648
1.40272

1.43074
1.76139
2.05156

2.14334
2.51815
2.85287

3.03750
3.44235
3.81093

0

0.5

50
100
200

10
20
30

0.52068
0.72445
0.91095

0.88454
1.15682
1.39469

1.42294
1.75507
2.04613

2.13821
2.51379
2.84902

3.03395
3.43921
3.80810

0

1

50
100
200

10
20
30

0.45095
0.67608
0.87298

0.84560
1.12732
1.37033

1.39930
1.73595
2.02976

2.12275
2.50066
2.83744

3.02325
3.42978
3.79959

1

0

0

0

0.18268

0.40836

0.70640

1.03105

1.36074

1

0

50
100
200

10
20
30

0.53582
0.73541
0.91969

0.85004
1.13066
1.37307

1.24680
1.61555
1.92780

1.67638
2.13482
2.52096

2.11541
2.66426
3.12598

1

0.5

50
100
200

10
20
30

0.51431
0.71989
0.90733

0.83673
1.12068
1.36487

1.23785
1.60865
1.92202

1.66982
2.12967
2.51660

2.11030
2.66021
3.12253

1

1

50
100
200

10
20
30

0.44359
0.67119
0.86920

0.79546
1.09021
1.33997

1.21059
1.58777
1.90458

1.64998
2.11415
2.50348

2.09490
2.64801
3.11214

2

0

0

0

0.16926

0.35404

0.57741

0.80843

1.03768

2

0

50
100
200

10
20
30

0.53139
0.73219
0.91712

0.82532
1.11219
1.35791

1.17852
1.56346
1.88435

1.54944
2.03666
2.43839

1.92357
2.51465
2.99949

2

0.5

50
100
200

10
20
30

0.50970
0.71660
0.90473

0.81160
1.10205
1.34962

1.16904
1.55633
1.87844

1.54234
2.03126
2.43388

1.91795
2.51035
2.9959

2

1

50
100
200

10
20
30

0.43823
0.66766
0.86647

0.76898
1.07105
1.32442

1.14014
1.53474
1.86060

1.52084
2.01498
2.42031

1.90099
2.49742
2.98506

3

0

0

0

0.15843

0.31687

0.50032

0.68689

0.87128

3

0

50
100
200

10
20
30

0.52804
0.72976
0.91518

0.81007
1.10092
1.34870

1.14273
1.53666
1.86218

1.48964
1.99154
2.40083

1.83915
2.45067
2.94606

3

0.5

50
100
200

10
20
30

0.50620
0.71412
0.90276

0.79609
1.09068
1.34035

1.13295
1.52940
1.85620

1.48225
1.98602
2.39625

1.83327
2.44626
2.94239

3

1

50
100
200

10
20
30

0.43416
0.66500
0.86442

0.75259
1.05935
1.31498

1.10311
1.50743
1.83813

1.45986
1.96937
2.38247

1.81552
2.43299
2.93137

Fig. 2. Natural frequencies $\omega $ vs the nonlocal parameter $\xi $
a) Damping coefficients ${c}_{t}$
b) Foundation parameters ${k}_{1}$ and ${k}_{2}$
c) Aspect ratios $a/b$
d) Mode numbers $m$ and $n$
Fig. 3. Natural frequencies $\omega $ vs the damping coefficient ${c}_{t}$
a) Nonlocal parameters $\xi $
b) Foundation parameters ${k}_{1}$ and ${k}_{2}$
c) Aspect ratios $a/b$
d) Mode numbers $m$ and $n$
Fig. 4. Natural frequencies $\omega $ vs the mode number $n$
a) Nonlocal parameters $\xi $
b) Foundation parameters ${k}_{1}$ and ${k}_{2}$
c) Damping coefficients ${c}_{t}$
d) Aspect ratios $a/b$
Fig. 5. Natural frequencies $\omega $ vs Pasternak’s parameter ${k}_{2}$
a) Nonlocal parameters $\xi $
b) Winkler’s parameters ${k}_{1}$
c) Aspect ratios $a/b$
d) Mode numbers $m$ and $n$
Fig. 4 shows the natural frequencies $\omega $ vs the mode number $n$ for different nonlocal parameters $\xi $, foundation parameters ${k}_{1}$ and ${k}_{2}$, damping coefficients ${c}_{t}$, and aspect ratios $a/b$. The frequency $\omega $ increases as the mode number $n$ increases and this irrespective of the values of other parameters. The frequencies are increasing with the increase of the foundation parameters ${k}_{1}$ and ${k}_{2}$ and aspect ratio $a/b$ and are decreasing with the increase of the nonlocal parameter $\xi $ and damping coefficient ${c}_{t}$.
Fig. 5 shows the natural frequencies $\omega $ vs Pasternak’s parameter ${k}_{2}$ for different nonlocal parameters $\xi $, Winkler’s parameters ${k}_{1}$, aspect ratios $a/b$, and mode numbers $m$ and $n$. The frequency $\omega $ increases as ${k}_{2}$ increases and this irrespective of the values of other parameters. The frequency is increasing with the increase of Winkler’s parameter ${k}_{1}$, aspect ratio $a/b$ and mode numbers $m$ and $n$ while it is decreasing with the increase of the nonlocal parameter $\xi $.
Finally, Fig. 6 plots the natural frequencies $\omega $ vs the aspect ratio $a/b$ for different nonlocal parameters $\xi $, foundation parameters ${k}_{1}$ and ${k}_{2}$, damping coefficients ${c}_{t}$, and mode numbers $m$ and $n$. The frequency $\omega $ is no longer decreasing as the aspect ratio $a/b$ increases and it has minimum values according to the values of other parameters. The frequencies are increasing with the increase of the foundation parameters ${k}_{1}$ and ${k}_{2}$ and mode numbers $m$ and $n$ and are decreasing with the increase of the nonlocal parameter $\xi $ and damping coefficient ${c}_{t}$.
5. Conclusions
In this article, a singlelayered graphene sheet is embedded in a threeparameter viscoelastic medium. The vibration frequency analysis is performed due to the nonlocal elasticity theory. For the sake of completeness and comparisons, some frequencies are tabulated here for different viscous damping coefficient, nonlocal parameter, aspect ratio, mode numbers, and WinklerPasternak’s elastic foundation. This article gives accurate frequencies as compared with the corresponding ones in the literature. The variation of frequency is highly sensitive to the variation of the different parameters. The maximum frequency occurs when the SLGS is embedded in twoparameter foundation medium without damping coefficient and with very low nonlocal parameter. In fact, the frequencies may be vanished for higher values of the viscous damping coefficient.
References
 Stankovich S., Dikin D. A., Dommett G. H. B., Kohlhaas K. M., Zimney E. J., Stach E. A., et al. Graphenebased composite materials. Nature, Vol. 442, 2006, p. 282286. [Publisher]
 Ramanathan T., Abdala A. A., Stankovich S., Dikin D. A., HerreraAlonso M., Piner R. D., et al. Functionalized graphene sheets for polymer nanocomposites. Nature Nanotechnology, Vol. 3, 2008, p. 327331. [Publisher]
 SakhaeePour A., Ahmadian M. T., Vafai A. Applications of singlelayered graphene sheets as mass sensors and atomistic dust detectors. Solid State Communications, Vol. 4, 2008, p. 168172. [Publisher]
 Kitipornchai S., He X. Q., Liew K. M. Continuum model for the vibration of multilayered graphene sheets. Physical Review B, Vol. 72, 2005, p. 075443. [Publisher]
 Behfar K., Naghdabadi R. Nanoscale vibrational analysis of a multilayered graphene sheet embedded in an elastic medium. Composites Science and Technology, Vol. 65, 2005, p. 11591164. [Publisher]
 Natsuki T., Endo M. Vibration analysis of embedded carbon nanotubes using wave propagation approach. Journal of Applied Physics, Vol. 99, 2006, p. 034311. [Publisher]
 Wang C. M., Tan V. B. C., Zhang Y. Y. Timoshenko beam model for vibration analysis of multiwalled carbon nanotubes. Journal of Sound and Vibration, Vol. 294, 2006, p. 10601072. [Publisher]
 Wang L., Ni Q. On vibration and instability of carbon nanotubes conveying fluid. Computational Materials Science, Vol. 43, 2008, p. 399402. [Publisher]
 Wang L., Ni Q., Li M., Qian Q. The thermal effect on vibration and instability of carbon nanotubes conveying fluid. Physica E, Vol. 40, 2008, p. 31793182. [Publisher]
 Ansari R., Hemmatnezhad M. Nonlinear vibrations of embedded multiwalled carbon nanotubes using a variational approach. Mathematical and Computer Modelling, Vol. 53, 2011, p. 927938. [Publisher]
 Ansari R., Hemmatnezhad M., Rezapour J. The thermal effect on nonlinear oscillations of carbon nanotubes with arbitrary boundary conditions. Current Applied Physics, Vol. 11, 2011, p. 692697. [Publisher]
 Akgöz B., Civalek Ö. Free vibration analysis for singlelayered graphene sheets in an elastic matrix via modified couple stress theory. Materials and Design, Vol. 42, 2012, p. 164171. [Publisher]
 Eringen A. C., Edelen D. G. B. On nonlocal elasticity. International Journal of Engineering Science, Vol. 10, 1972, p. 233248. [Publisher]
 Eringen A. C. Nonlocal polar elastic continua. International Journal of Engineering Science, Vol. 10, 1972, p. 116. [Publisher]
 Eringen A. C. On differential equations of nonlocal elasticity and solutions of screw dislocation and surface waves. Journal of Applied Physics, Vol. 54, 1983, p. 47034710. [Publisher]
 Eringen A. C. Nonlocal Continuum Field Theories. Springer Verlag, New York, 2002. [Search CrossRef]
 Peddieson J., Buchanan G. R., McNitt R. P. Application of nonlocal continuum models to nanotechnology. International Journal of Engineering Science, Vol. 41, 2003, p. 305312. [Publisher]
 Wang Q., Varadan V. K. Vibration of carbon nanotubes studied using nonlocal continuum mechanics. Smart Materials and Structures. Vol. 15, 2006, p. 659666. [Publisher]
 Li R., Kardomateas G. A. Vibration characteristics of multiwalled carbon nanotubes embedded in elastic media by a nonlocal elastic shell model. Journal of Applied Mechanics, Vol. 74, 2007, p. 10871094. [Publisher]
 Xu K. Y., Aifantis E. C., Yan Y. H. Vibrations of doublewalled carbon nanotubes with different boundary conditions between inner and outer tubes. Journal of Applied Mechanics, Vol. 75, 2008, p. 021013. [Publisher]
 Aydogdu M. Axial vibration of the nanorods with the nonlocal continuum rod model. Physica E, Vol. 41, 2009, p. 861864. [Publisher]
 Pradhan S. C., Phadikar J. K. Small scale effect on vibration of embedded multilayered graphene sheets based on nonlocal continuum models. Physics Letters A, Vol. 373, 2009, p. 10621069. [Publisher]
 Pradhan S. C., Phadikar J. K. Nonlocal elasticity theory for vibration of nanoplates. Journal of Sound and Vibration, Vol. 325, 2009, p. 206223. [Publisher]
 Murmu T., Pradhan S. C. Vibration analysis of nanosinglelayered graphene sheets embedded in elastic medium based on nonlocal elasticity theory. Journal of Applied Physics, Vol. 105, 2009, p. 064319. [Publisher]
 Pradhan S. C., Murmu T. Smallscale effect on vibration analysis of singlewalled carbon nanotubes embedded in an elastic medium using nonlocal elasticity theory. Journal of Applied Physics, Vol. 105, 2009, p. 124306. [Publisher]
 Arash B., Ansari R. Evaluation of nonlocal parameter in the vibrations of singlewalled carbon nanotubes with initial strain. Physica E, Vol. 42, 2010, p. 20582064. [Publisher]
 Ansari R., Sahmani S., Arash B. Nonlocal plate model for free vibrations of singlelayered graphene sheets. Physics Letters A, Vol. 375, 2010, p. 5362. [Publisher]
 Pradhan S. C., Kumar A. Vibration analysis of orthotropic graphene sheets embedded in Pasternak elastic medium using nonlocal elasticity theory and differential quadrature method. Computational Materials Science, Vol. 50, 2010, p. 239245. [Publisher]
 Pradhan S. C., Kumar A. Vibration analysis of orthotropic graphene sheets using nonlocal elasticity theory and differential quadrature method. Composite Structures, Vol. 93, 2011, p. 774779. [Publisher]
 Ansari R., Arash B., Rouhi H. Vibration characteristics of embedded multilayered graphene sheets with different boundary conditions via nonlocal elasticity. Composite Structures, Vol. 93, 2011, p. 24192429. [Publisher]
 Wang C. Y., Murmu T., Adhikari S., Mechanisms of nonlocal effect on the vibration of nanoplates. Applied Physics Letters, Vol. 98, 2011, p. 153101. [Publisher]
 Shen Z.B., Tang H.L., Li D.K., Tang G.J. Vibration of singlelayered graphene sheetbased nanomechanical sensor via nonlocal Kirchhoff plate theory. Computational Materials Science, Vol. 61, 2012, p. 200205. [Publisher]
 Natsuki T., Shi J.X., Ni Q.Q. Vibration analysis of circular doublelayered graphene sheets. Journal of Applied Physics, Vol. 111, 2012, p. 044310. [Publisher]
 Zenkour A. M., Sobhy M. Nonlocal elasticity theory for thermal buckling of nanoplates lying on WinklerPasternak elastic substrate medium. Physica E, Vol. 53, 2013, p. 251259. [Publisher]
 Zenkour A. M., Abouelregal A. E. Vibration of FG nanobeams induced by sinusoidal pulseheating via a nonlocal thermoelastic model. Acta Mechanica, Vol. 225, 2014, p. 34093421. [Publisher]
 Mandal U., Pradhan S. C. Transverse vibration analysis of singlelayered graphene sheet under magnetothermal environment based on nonlocal plate theory. Journal of Applied Physics, Vol. 116, 2014, p. 164303. [Publisher]
 Zenkour A. M., Abouelregal A. E. The effect of two temperatures on a FG nanobeam induced by a sinusoidal pulse heating. Structural Engineering and Mechanics, Vol. 51, 2014, p. 199214. [Publisher]
 Asemi S. R., Farajpour A. Thermoelectromechanical vibration of coupled piezoelectric nanoplate systems under nonuniform voltage distribution embedded in Pasternak elastic medium. Current Applied Physics, Vol. 14, 2014, p. 814832. [Publisher]
 Zenkour A. M., Abouelregal A. E. Nonlocal thermoelastic nanobeam subjected to a sinusoidal pulse heating and temperaturedependent physical properties, Microsystem Technologies, Vol. 21, 2015, p. 17671776. [Publisher]
 Zhang Y., Lei Z. X., Zhang L. W., Liew K. M., Yu J. L. Nonlocal continuum model for vibration of singlelayered graphene sheets based on the elementfree kpRitz method. Engineering Analysis with Boundary Elements, Vol. 56, 2015, p. 9097. [Publisher]
 Zenkour A. M., Abouelregal A. E., Alnefaie K. A., Zhang X., Aifantis E. C. Nonlocal thermoelasticity theory for thermalshock nanobeams with temperaturedependent thermal conductivity. Journal of Thermal Stresses, Vol. 38, 2015, p. 10491067. [Publisher]
 Zenkour A. M., Abouelregal A. E., Alnefaie K. A., Aljinaidi A. A., AbuHamdeh N. H., Aifantis E. C. State space approach for the vibration of nanobeams based on the nonlocal thermoelasticity theory without energy dissipation. Journal of Mechanical Science and Technology, Vol. 29, 2015, p. 29212931. [Publisher]
 Karličić D., Cajic M., Kozić P., Pavlović I. Temperature effects on the vibration and stability behavior of multilayered graphene sheets embedded in an elastic medium. Composite Structures, Vol. 131, 2015, p. 672681. [Publisher]
 Arani A. G., Shiravand A., Rahi M., Kolahchi R. Nonlocal vibration of coupled DLGS systems embedded on viscoPasternak foundation. Physica B, Vol. 407, 2012, p. 41234131. [Publisher]
 Pouresmaeeli S., Ghavanloo E., Fazelzadeh S. A. Vibration analysis of viscoelastic orthotropic nanoplates resting on viscoelastic medium. Composite Structures, Vol. 96, 2013, p. 405410. [Publisher]
 Mohammadi M., Farajpour A., Goodarzi M., Mohammadi H. Temperature effect on vibration analysis of annular graphene sheet embedded on viscoPasternak foundation. Journal of Solid Mechanics, Vol. 5, 2013, p. 305323. [Search CrossRef]
 Karličić D., Kozić P., Pavlović R. Free transverse vibration of nonlocal viscoelastic orthotropic multinanoplate system (MNPS) embedded in a viscoelastic medium. Composite Structures, Vol. 115, 2014, p. 8999. [Publisher]
 Goodarzi M., Mohammadi M., Farajpour A., Khooran M. Investigation of the effect of prestressed on vibration frequency of rectangular nanoplate based on a viscoPasternak foundation. Journal of Solid Mechanics, Vol. 6, 2014, p. 98121. [Search CrossRef]
 Hashemi Sh. H., Mehrabani H., AhmadiSavadkoohi A. Exact solution for free vibration of coupled double viscoelastic graphene sheets by viscoPasternak medium. Composites Part B, Vol. 78, 2015, p. 377383. [Publisher]
 Zenkour A. M. Nonlocal transient thermal analysis of a singlelayered graphene sheet embedded in viscoelastic medium. Physica E, Vol. 79, 2016, p. 8797. [Publisher]
Cited By
Lecture Notes in Mechanical Engineering
Harshad Patel, Saumil Desai, Mitesh B. Panchal

2021

Acta Mechanica
ChihPing Wu, HaoXiang Hu

2021

International Journal of Structural Stability and Dynamics
Iqbal Kaur, Parveen Lata, Kulvinder Singh

2020

Acta Mechanica
Mohammad Arefi, Ashraf M. Zenkour

2017

Composite Structures
Mohammad Arefi, Ashraf M. Zenkour

2017

Physica B: Condensed Matter
Mohammad Arefi, Ashraf M. Zenkour

2017

Journal of Thermal Stresses
Ashraf M. Zenkour, Mohammad Arefi

2017

Mechanics Research Communications
Mohammad Arefi, Ashraf M. Zenkour

2017

Smart Materials and Structures
Mohammad Arefi, Ashraf M Zenkour

2016

Advances in nano research
Ashraf M. Zenkour

2016

Mathematical Modelling and Analysis
Ashraf M. Zenkour

2016
